Today's standard for tomorrow's materials. © MAY 2019 NANOVEA
Wood has been used for thousands of years as a building material for homes, furniture and ooring. It has a combination of natural beauty, durability and restorability, making it an ideal candidate for ooring. Unlike carpet, hardwood oors keep their color for a long time and can be easily cleaned and maintained, however, being a natural material, most wood ooring requires the application of a surface nish to protect the wood from various kinds of damage such as scung and chipping over time. In this study, a Nanovea Tribometer was used to measure the wear rate and coecient of friction (COF) to better under- stand the comparative performance of three wood nishes.[email protected] [email protected]
Importance of Comparing Wood Finish Wear & COF
The service behavior of a wood species used for ooring is often related to its wear resistance. The change in the individual cellular and ber structure of dierent species of wood contributes to their dierent mechani- cal and tribological behaviors. Actual service tests of wood as ooring materials are expensive, dicult to duplicate, and require long periods of testing time. As a result, it becomes valuable to develop a simple wear test that can produce reliable, reproducible, and straight forward.
Versatile Wear & Friction Tester
Robust with Open Platform
Wide Range of Environmental Conditions
Learn More about the T50
In this study, we simulated and compared the wear behaviors of three types of wood to showcase the capability of the Nanovea Tribometer in evaluating the tribological properties of wood in a controlled and monitored manner.
Sample Description: Antique Birch Hardwood has a 7-layer aluminum oxide nish, providing everyday wear and tear protection. Courtship Grey Oak, & Santos Mahogany are both laminate ooring types that vary in surface nish and gloss. The Courtship Grey Oak is a slate gray color, EIR nish, and low gloss. On the other hand, Santos Mahogany is a dark burgundy color, prenished, and high gloss which allows surface scratches and defects to be more easily hidden.
The evolution of COF during the wear tests of the three wood ooring samples are plotted in Fig. 1. The Antique Birch Hardwood, Courtship Grey Oak, & Santos Mahogany samples all showed dierent COF behavior.
It can be observed in the graph above that Antique Birch Hardwood was the only sample that demonstrated a steady COF for the duration of an entire test. The Courtship Grey Oak’s sharp increase in COF and then gradual decrease could be indicative that the sample’s surface roughness largely contributed to its COF behavior. As the sample wore, the surface roughness decreased and became more homogenous which explain the decrease in COF as the sample surface became smoother from mechanical wear. The COF on Santos Mahoga- ny displays a smooth gradual increase in COF at the beginning of the test and then transitioned abruptly into a choppy COF trend. This could indicate that once the laminate coating started to wear through, the steel ball (counter material) made contact with the wood substrate which wore at a quicker and turbulent manner creating the noisier COF behavior towards the end of the test.
Instrument T50 Wood Samples Antique Birch Hardwood,
Courtship Grey Oak, & Santos Mahogany
Normal Force (N) 20 Wear ring Radius (mm) 6 Speed (RPM) 300 Duration of Test (minutes) 10
Sample of Antique Birch, Courtship Grey Oak, and Santos Mahogany (left to right)
Antique Birch Hardwood
Figure 2: 3D view of scan taken for Sample Antique Birch Hardwood
Figure 3: Volume of a Hole
Sample of Antique Birch
Courtship Grey Oak
Figure 4: 3D view of scan taken for Sample Courtship Grey Oak
Figure 5: Volume of a Hole
Sample of Courtship Grey Oak
Figure 6: 3D view of scan taken for Sample Santos Mahogany
Figure 7: Volume of a Hole
Table 2: Result Summary of the wear track analysis.
Table 2 summarizes the results of the wear track scans and analysis on all wood ooring samples after the wear tests were performed. Detailed information and images for each sample can be seen in Figures 2-7. Based on the Wear Rate comparison between all three samples, we can deduct that Santos Mahogany proved to be less resilient to mechanical wear than the other two samples. Antique Birch Hardwood and Courtship Grey Oak had very similar wear rates although their wear behavior during the course of their tests diered signicantly. Antique Birch Hardwood had a gradual and more uniform wear trend while Court- ship Grey Oak showed a shallow and pitted wear track due to the pre-existing surface texture and nish
Sample Volume Lost (µm³) Wear Rate x10-5 (mm3/Nm)
Antique Birch Hardwood 419852848 18.58 Courtship Grey Oak 422305079 18.69
Santos Mahogany 1.95E+10 862.86
In this study, we showcased the capacity of Nanovea’s Tribometer in evaluating the coecient of friction and wear resistance of three types of wood, Antique Birch Hardwood, Courtship Grey Oak, and Santos Mahogany in a controlled and monitored manner. The superior mechanical properties of the Antique Birch Hardwood leads to its better wear resistance. The texture and homogeneity of the wood surface plays an important role in the wear behavior. The Courtship Grey Oak surface texture such as gaps or cracks between the wood cell bers may become the weak spots where the wear initiates and propagates.
Check out our full application notes library!
A Better Measure [email protected]
Thank you for reading!
We appreciate your interest in our technology and services. Read more about all of our product line and lab services at www.nanovea.com
Call to Schedule a demo today!
If you have any questions please email us at [email protected][email protected] [email protected]
Check out our other application note where we conduct a Viscoelastic Analysis on Rubber with Nanoindentation